Amination of energetic anions: high-performing energetic materials.
Klapötke, Thomas M; Piercey, Davin G.; Stierstorfer, Jörg; Dalton transactions (Cambridge, England : 2003) 41 (2012) 9451–9459; doi:10.1039/c2dt30684k

data_7019821
_publ_section_title
;
 Amination of energetic anions: high-performing energetic materials.
;
_journal_issue                   31
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9451
_journal_page_last               9459
_journal_paper_doi               10.1039/c2dt30684k
_journal_volume                  41
_journal_year                    2012
_chemical_formula_moiety         'C2 H2 N6 O4'
_chemical_formula_sum            'C2 H2 N6 O4'
_chemical_formula_weight         174.10
_chemical_name_common            1-amino-3,5-dinitro-1,2,4-triazole
_chemical_name_systematic        1-amino-3,5-dinitro-1,2,4-triazole
_space_group_IT_number           1
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date
;
'Tue Sep 06 13:04:56 2011'
;
_audit_creation_method
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.11 (release 16-05-2011 CrysAlis171 .NET)
(compiled May 16 2011,17:55:39)
;
_audit_update_record             10.05.2012
_cell_angle_alpha                78.074(8)
_cell_angle_beta                 77.335(8)
_cell_angle_gamma                89.873(6)
_cell_formula_units_Z            8
_cell_length_a                   8.3125(7)
_cell_length_b                   11.4102(8)
_cell_length_c                   13.5629(16)
_cell_measurement_reflns_used    3066
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      32.2309
_cell_measurement_theta_min      4.2424
_cell_volume                     1226.8(2)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.11 (release 16-05-2011 CrysAlis171 .NET)
(compiled May 16 2011,17:55:39)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.11 (release 16-05-2011 CrysAlis171 .NET)
(compiled May 16 2011,17:55:39)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.11 (release 16-05-2011 CrysAlis171 .NET)
(compiled May 16 2011,17:55:39)
;
_computing_molecular_graphics
;
'ORTEP (M. N. Burnett, C. K. Johnson, ORTEP-III: Oak Ridge Thermal Ellipsoid
;
_computing_publication_material
'PLATON (A. L. Spek, Acta Crystallogr, Sect. A, 1990, 46, C34, 1995 version).'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    SIR-92
_diffrn_ambient_temperature      173
_diffrn_detector_area_resol_mean 15.9809
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device       'CCD camera on \k-goniostat'
_diffrn_measurement_device_type  'Xcalibur, Sapphire3'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_UB_11      0.0791337000
_diffrn_orient_matrix_UB_12      0.0229526000
_diffrn_orient_matrix_UB_13      -0.0294427000
_diffrn_orient_matrix_UB_21      0.0204336000
_diffrn_orient_matrix_UB_22      0.0124658000
_diffrn_orient_matrix_UB_23      0.0450052000
_diffrn_orient_matrix_UB_31      0.0313790000
_diffrn_orient_matrix_UB_32      -0.0579892000
_diffrn_orient_matrix_UB_33      0.0107311000
_diffrn_radiation_collimation    0.5
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Enhance (Mo) X-ray Source'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0303
_diffrn_reflns_av_sigmaI/netI    0.0455
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            9699
_diffrn_reflns_theta_full        26.49
_diffrn_reflns_theta_max         26.49
_diffrn_reflns_theta_min         4.25
_diffrn_source_current           40
_diffrn_source_type              'Spellman generator'
_diffrn_source_voltage           50
_exptl_absorpt_coefficient_mu    0.177
_exptl_absorpt_correction_T_max  0.9825
_exptl_absorpt_correction_T_min  0.9570
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.11 (release 16-05-2011 CrysAlis171 .NET)
(compiled May 16 2011,17:55:39)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.885
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       rod
_exptl_crystal_F_000             704
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.254
_refine_diff_density_min         -0.256
_refine_diff_density_rms         0.047
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.2(10)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     913
_refine_ls_number_reflns         5066
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.020
_refine_ls_R_factor_all          0.0442
_refine_ls_R_factor_gt           0.0344
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0368P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0709
_refine_ls_wR_factor_ref         0.0769
_reflns_number_gt                4379
_reflns_number_total             5066
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2dt30684k.txt
_cod_data_source_block           gx516
_cod_original_sg_symbol_Hall     P1
_cod_database_code               7019821